Advancement in Electrospun Nanofibrous Membranes ... membranes were exploited for the first three...
Embed Size (px)
Transcript of Advancement in Electrospun Nanofibrous Membranes ... membranes were exploited for the first three...
Membranes 2013, 3, 266-284; doi:10.3390/membranes3040266
membranes ISSN 2077-0375
Advancement in Electrospun Nanofibrous Membranes Modification and Their Application in Water Treatment
Shaik Anwar Ahamed Nabeela Nasreen 1,*, Subramanian Sundarrajan 2,*, Syed Abdulrahim Syed Nizar 1, Ramalingam Balamurugan 1 and Seeram Ramakrishna 1, 2,*
1 NUS Nanoscience and Nanotechnology Institute, National University of Singapore, 2 Engineering Drive 3, 117581, Singapore
2 Department of Mechanical Engineering, National University of Singapore, 2 Engineering Drive 3, 117575, Singapore
* Authors to whom correspondence should be addressed; E-Mails: email@example.com (S.A.A.N.N.); firstname.lastname@example.org (S.S.); email@example.com (S.R.); Tel.: +65-6516-4272 (S.R.); Fax: +65-6773-0339 (S.R.).
Received: 3 September 2013 / Accepted: 13 September 2013 / Published: 30 September 2013
Abstract: Water, among the most valuable natural resources available on earth, is under serious threat as a result of undesirable human activities: for example, marine dumping, atmospheric deposition, domestic, industrial and agricultural practices. Optimizing current methodologies and developing new and effective techniques to remove contaminants from water is the current focus of interest, in order to renew the available water resources. Materials like nanoparticles, polymers, and simple organic compounds, inorganic clay materials in the form of thin film, membrane or powder have been employed for water treatment. Among these materials, membrane technology plays a vital role in removal of contaminants due to its easy handling and high efficiency. Though many materials are under investigation, nanofibers driven membrane are more valuable and reliable. Synthetic methodologies applied over the modification of membrane and its applications in water treatment have been reviewed in this article.
Keywords: electrospinning; nanofibers; synthesis; surface modification; interfacial polymerization; heavy metal; antibacterial
Membranes 2013, 3 267
Nanoparticles, nanofibers and other nanostructures bring tremendous technological advancements in the field of electronics , catalysis , bioengineering  and environmental applications . Such nanostructures using various materials such as polymeric , inorganic metal/polymer composite  with variations in their composition, configuration and assembly have been produced by various techniques such as electrospinning , template assisted synthesis , phase separation , self assembly , solvent evaporation , drawing-processing method  and doctor blading method . Among them, electrospinning is one of the most versatile and simple techniques, which has been applied to fabricate one dimensional nanostructures viz., nanofibers. Recently, numerous journal articles have documented electrospun nanofibrous “Membranes” (ENMs) for water treatment applications. A review article by Balamurugan et al.  reports on recent trends in nanofibrous membranes and their suitability for air and water filtration applications, preparation and characterization of electrospun nanofibers membranes and their possible applications in water treatment. Feng et al.  and Subramanian et al.  report on “New Directions of nanofibers in nanofiltration applications”. These are some of very recent reports which emphasize the importance of ENMs in water technology.
ENMs have unique and interesting features, such as high surface area to volume ratio, large porosity, good mechanical properties and good water permeability, which provides a major contribution towards water treatment. These nanofibers were employed for the various water treatment applications based on their thickness, porosity, and surface roughness. The most widely applied filtration methods are microfiltration , ultrafiltration , nanofiltration , reverse osmosis  and forward osmosis and pressure retarded osmosis . Among them, electrospun nanofiber membranes were exploited for the first three applications, which are covered in this review.
2. Nanofiber Preparation—Electrospinning Technique
Electrospinning is a versatile technique for manufacturing of nanofibers with different diameter and varied morphologies. Ultrafine nanofibers from micro to nano scale can be produced with ease. Solution viscosity, applied voltage range, humidity, tip to the collector distance are some of the important parameters that governs the formation of nanofibers. Variations in the above mentioned parameters will result in formation of thin to thick nanofibers and smooth to corrugated surfaces. A simple diagram of the electrospinning set up is shown in Figure 1.
In this process, a high voltage is applied to create an electrically charged jet of polymer solution from a syringe. The voltage is applied gradually and when the applied voltage overcomes the surface tension of the polymer solution, a Taylor cone appears and it spins down as a fiber to reach the collector plate. Before reaching the collector, the solvent evaporates and the polymer solidifies and gets collected as fibers. One end of the supply is connected to a syringe needle and the other to the collector that is grounded. Solution from the jet which is held by the surface tension will overcome once induces a charge on the surface of the liquid. Repulsion and contraction of the surface charges to the counter electrode cause a force directly opposite to the surface tension. As the voltage increased, the Taylor cone formed from the tip of needle surface elongates, i.e., the fluid elongates to attain a
Membranes 2013, 3 268
critical value where the repulsive force overcomes the surface tension and discharge. The discharged polymer solution jet undergoes an instability and elongation process, which allows the jet to become very long, uniform and thin fibers.
Although electrospinning is a methodology with numerous potential in various applications, one of the main disadvantages is the disability to achieve large scale productivity. Recently, multijet  and needless electrospinning techniques  are emerging to bridge the gap of large scale manufacturing.
Figure 1. Electrospinning set up.
3. Modifications of Electrospun Nanofiber Membranes (ENMs)
3.1. Surface Modification of ENMs
Electrospun nanofibers are being synthesized at an increasing rate to meet its demand for various applications. Many different methods of synthesis of polymer for electrospinning to the targeted applications are available. The established methods include sol-gel synthesis , in situ polymerization , surface modification , plasma induced grafting , Graft polymerization , blending , polymer-inorganic composites formation techniques , etc. The resultant physical morphology and mechanical properties vary depending on the polymeric concentration and spinning condition employed during the process. Selectivity in contaminant removal, mechanical strength, and porosity of the polymer network can be modified in the ENMs in order to improve their performances towards water purification. The surface modifications of the ENMs enhance the nanofibers matrix properties such as availability of functional groups on the surface of nanofibers. Some of the other surface modification techniques are oxidation process , plasma treatment , solvent vapor treatment  and surface coating .
Cellulose, a biopolymer made nanofibers is commonly used as adsorbent for the water filtration studies. The optimal required capacity of the cellulose fiber was not attainable, due to its low surface
Membranes 2013, 3 269
area and stability. Synthetic modifications of the cellulose materials with organic functional groups are very important in order to improve the polymers activity with the pollutant either by adsorption or sensing. Stephen et al.  modified nanofibers with oxolone-2,5-dione, which not only enhanced the surface area of the nanofiber mat and also helped in detecting heavy metals like cadmium and lead. The adsorption capacities based on time studies of these membranes (Figure 2) were compared with commercial adsorbents such as Dowex and Amberlite resin. They also suggested that these modified nanofibers membranes can be regenerated by treating with nitric acid and reused.
Figure 2. Effect of contact time on adsorption: (A) Pb and (B) Cd (I: cellulose and II: cellulose-g-oxolane-2,5-dione nanofibers). (Reprinted with permission from . Copyright 2011 Elsevier).
The modification of chitosan fibers was conducted by Schiffman et al. by crosslinking  using Glutaratldehyde and shciffs imine. Followed by Schiffman, Haider et al.  reported the solubility of chitosan nanofibers by treatment with trifluoroacetic acid (TFA). TFA forms a salt and exists in the form of ammonium cation and trifluoroacetate anion in the fibers. The amine group of chitosan was made available when this nanofiber was subjected to base treatment with K2CO3. The potassium cation binds with acetate and undergoes neutralization. This neutralization has allowed free amine group, which preferred to absorb more heavy metals. The salts helped the nanofiber mats to remain stable in aqueous medium to remove the contaminants. They reported that Cu (II) adsorption of nanofibers were ~6 and ~11 times higher than chitosan microsphere (80.71 mg/g) and the plain chitosan (45.20 mg/g), respectively.
Nanofiber template assiste